#------------------------------------------------------------------------------
#$Date: 2018-01-15 16:48:11 +0200 (Mon, 15 Jan 2018) $
#$Revision: 205229 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/32/19/4321991.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4321991
loop_
_publ_author_name
'Matthew A. Withersby'
'Alexander J. Blake'
'Neil R. Champness'
'Paul A. Cooke'
'Peter Hubberstey'
'Wan-Sheung Li'
'Martin Schröder'
_publ_section_title
;
 Solvent Control in the Synthesis of
 3,6-Bis(pyridin-3-yl)-1,2,4,5-tetrazine-Bridged Cadmium(II) and Zinc(II)
 Coordination Polymers
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              2259
_journal_page_last               2266
_journal_paper_doi               10.1021/ic980898h
_journal_volume                  38
_journal_year                    1999
_chemical_compound_source
;
?
;
_chemical_formula_moiety         ' C19 H16 Zn1 N11 O7 '
_chemical_formula_sum            'C19 H16 N11 O7 Zn'
_chemical_formula_weight         575.79
_chemical_melting_point          ?
_chemical_name_systematic
;
 {[Zn2(3,6-bis(pyridin-3-yl)-1,2,4,5-tetrazine)2(NO3)4(MeOH)2
(mu-3,6-bis(pyridin-3-yl)-1,2,4,5-tetrazine)]}n
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_audit_creation_date             98-03-25
_audit_creation_method           CRYSTALS
_cell_angle_alpha                85.36(1)
_cell_angle_beta                 80.63(1)
_cell_angle_gamma                69.34(1)
_cell_formula_units_Z            2
_cell_length_a                   7.535(1)
_cell_length_b                   10.728(1)
_cell_length_c                   15.219(2)
_cell_measurement_reflns_used    60
_cell_measurement_temperature    150.0(2)
_cell_measurement_theta_max      17.5
_cell_measurement_theta_min      12.5
_cell_volume                     1135.4(3)
_computing_cell_refinement       'STADI4 (Stoe & Cie 1995a)'
_computing_data_collection       'STADI4 (Stoe & Cie 1995a)'
_computing_data_reduction
;
X-RED (Stoe & Cie, 1995b)
CRYSTALS (Watkin et al, 1996)
;
_computing_molecular_graphics    'CAMERON (Watkin, Prout and Pearce, 1996)'
_computing_publication_material
;
CRYSTALS Issue 10 (Watkin et al, 1996)
;
_computing_structure_refinement
;
CRYSTALS Issue 10 (Watkin et al, 1996)
;
_computing_structure_solution    'SIR92 (Altomare, et al, 1994)'
_diffrn_ambient_temperature      150
_diffrn_measurement_device       'STOE STADI4 4-circle diffractometer D092'
_diffrn_measurement_method       2θ/ω
_diffrn_radiation_detector       'NaI (Tl) scintillation counter'
_diffrn_radiation_monochromator  'planar graphite'
_diffrn_radiation_polarisn_norm  90.0
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.00
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            5257
_diffrn_reflns_theta_max         25.03
_diffrn_reflns_theta_min         2.71
_diffrn_standards_decay_%        4.00
_diffrn_standards_interval_time  '60 minutes'
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    1.171
_exptl_absorpt_correction_T_max  0.713
_exptl_absorpt_correction_T_min  0.613
_exptl_absorpt_correction_type   psi-scans
_exptl_crystal_colour            'red '
_exptl_crystal_density_diffrn    1.68
_exptl_crystal_description       'trapezoidal plate'
_exptl_crystal_F_000             586.54
_exptl_crystal_size_max          0.75
_exptl_crystal_size_mid          0.33
_exptl_crystal_size_min          0.10
_refine_diff_density_max         0.81
_refine_diff_density_min         -0.52
_refine_ls_extinction_method     None
_refine_ls_goodness_of_fit_all   1.0850
_refine_ls_goodness_of_fit_obs   1.0850
_refine_ls_number_parameters     407
_refine_ls_number_reflns         5092
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0439
_refine_ls_R_factor_obs          0.0439
_refine_ls_shift/esd_max         0.0055207
_refine_ls_structure_factor_coef F**2
_refine_ls_wR_factor_all         0.0633
_refine_ls_wR_factor_obs         0.0633
_reflns_limit_h_max              8
_reflns_limit_h_min              -8
_reflns_limit_k_max              12
_reflns_limit_k_min              -12
_reflns_limit_l_max              18
_reflns_limit_l_min              -16
_reflns_number_observed          5092
_reflns_number_total             5257
_reflns_observed_criterion       >2.00\s(I)
_cod_data_source_file            ic980898h_4.cif
_cod_data_source_block           CRYSTALS_cif
_cod_depositor_comments
;
The following automatic conversions were performed:

'_chemical_melting_point' value 'not measured' was changed to '?' -
the value is undefined or not given.

Automatic conversion script
Id: cif_fix_values 1673 2011-04-08 12:14:43Z adriana 

Setting the value of '_diffrn_ambient_temperature' to '150' as per
original publication.

Andrius Merkys
2018-01-15
;
_cod_original_cell_volume        1135.34
_cod_original_sg_symbol_H-M      'P -1 '
_cod_original_formula_sum        ' C19 H16 Zn1 N11 O7 '
_cod_database_code               4321991
loop_
_symmetry_equiv_pos_as_xyz
x,y,z
-x,-y,-z
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_occupancy
_atom_site_thermal_displace_type
ZN1 0.56750(4) 0.47543(3) 0.29196(2) 0.0208 1.0000 Uani
N101 0.3790(3) 1.0936(2) 0.5576(1) 0.0291 1.0000 Uani
N102 0.3073(3) 1.0275(2) 0.5119(2) 0.0283 1.0000 Uani
C103 0.4302(3) 0.9354(2) 0.4559(2) 0.0214 1.0000 Uani
N131 0.3940(3) 0.6649(2) 0.3287(1) 0.0220 1.0000 Uani
C132 0.4627(3) 0.7366(2) 0.3734(2) 0.0220 1.0000 Uani
C133 0.3489(3) 0.8619(2) 0.4051(2) 0.0188 1.0000 Uani
C134 0.1594(3) 0.9144(2) 0.3902(2) 0.0216 1.0000 Uani
C135 0.0914(3) 0.8408(2) 0.3436(2) 0.0240 1.0000 Uani
C136 0.2107(3) 0.7173(2) 0.3137(2) 0.0225 1.0000 Uani
N1 1.0672(3) 0.0598(2) -0.1234(1) 0.0238 1.0000 Uani
N2 0.9027(3) 0.1290(2) -0.0756(1) 0.0238 1.0000 Uani
C3 0.9096(3) 0.2067(2) -0.0133(2) 0.0190 1.0000 Uani
N4 1.0722(3) 0.2079(2) 0.0124(1) 0.0212 1.0000 Uani
N5 1.2363(3) 0.1359(2) -0.0333(1) 0.0210 1.0000 Uani
C6 1.2270(3) 0.0708(2) -0.1034(2) 0.0193 1.0000 Uani
N31 0.5570(3) 0.4116(2) 0.1680(1) 0.0204 1.0000 Uani
C32 0.7211(3) 0.3429(2) 0.1178(2) 0.0190 1.0000 Uani
C33 0.7251(3) 0.2886(2) 0.0371(2) 0.0188 1.0000 Uani
C34 0.5521(3) 0.3078(2) 0.0074(2) 0.0217 1.0000 Uani
C35 0.3835(4) 0.3778(3) 0.0593(2) 0.0262 1.0000 Uani
C36 0.3906(3) 0.4279(2) 0.1389(2) 0.0232 1.0000 Uani
N61 1.5795(3) -0.1592(2) -0.2733(1) 0.0253 1.0000 Uani
C62 1.4157(3) -0.0860(2) -0.2251(2) 0.0224 1.0000 Uani
C63 1.4108(3) -0.0031(2) -0.1584(2) 0.0191 1.0000 Uani
C64 1.5824(3) 0.0068(2) -0.1431(2) 0.0225 1.0000 Uani
C65 1.7510(3) -0.0671(2) -0.1934(2) 0.0239 1.0000 Uani
C66 1.7431(3) -0.1491(2) -0.2568(2) 0.0256 1.0000 Uani
N10 0.7937(3) 0.3067(2) 0.3933(1) 0.0234 1.0000 Uani
O11 0.6808(2) 0.4221(2) 0.4159(1) 0.0314 1.0000 Uani
O12 0.7833(2) 0.2677(2) 0.3189(1) 0.0291 1.0000 Uani
O13 0.9096(3) 0.2384(2) 0.4416(1) 0.0345 1.0000 Uani
N20 0.8202(3) 0.6094(2) 0.1938(1) 0.0232 1.0000 Uani
O21 0.8241(2) 0.5183(2) 0.2524(1) 0.0273 1.0000 Uani
O22 0.9600(2) 0.6465(2) 0.1745(1) 0.0365 1.0000 Uani
O23 0.6726(3) 0.6623(2) 0.1578(1) 0.0393 1.0000 Uani
O10 0.3477(2) 0.3992(2) 0.3421(1) 0.0293 1.0000 Uani
C11 0.2144(5) 0.4253(3) 0.4217(2) 0.0417 1.0000 Uani
H132 0.591(4) 0.694(3) 0.382(2) 0.029(7) 1.0000 Uiso
H134 0.085(4) 1.001(3) 0.412(2) 0.027(7) 1.0000 Uiso
H135 -0.035(4) 0.869(3) 0.331(2) 0.037(8) 1.0000 Uiso
H136 0.164(3) 0.665(2) 0.282(2) 0.013(6) 1.0000 Uiso
H32 0.829(4) 0.334(3) 0.137(2) 0.027(7) 1.0000 Uiso
H34 0.553(4) 0.272(3) -0.045(2) 0.027(7) 1.0000 Uiso
H35 0.273(4) 0.390(3) 0.041(2) 0.023(7) 1.0000 Uiso
H36 0.273(3) 0.471(2) 0.178(2) 0.021(6) 1.0000 Uiso
H62 1.310(4) -0.098(3) -0.236(2) 0.036(8) 1.0000 Uiso
H64 1.583(3) 0.065(3) -0.102(2) 0.022(7) 1.0000 Uiso
H65 1.864(4) -0.061(2) -0.184(2) 0.019(6) 1.0000 Uiso
H66 1.860(4) -0.206(3) -0.290(2) 0.031(7) 1.0000 Uiso
H10 0.375(4) 0.321(3) 0.327(2) 0.043(9) 1.0000 Uiso
H11 0.204(4) 0.355(3) 0.452(2) 0.048(9) 1.0000 Uiso
H12 0.222(4) 0.489(3) 0.455(2) 0.047(9) 1.0000 Uiso
H13 0.081(8) 0.468(5) 0.402(3) 0.13(2) 1.0000 Uiso
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_Cromer_Mann_a1
_atom_type_scat_Cromer_Mann_b1
_atom_type_scat_Cromer_Mann_a2
_atom_type_scat_Cromer_Mann_b2
_atom_type_scat_Cromer_Mann_a3
_atom_type_scat_Cromer_Mann_b3
_atom_type_scat_Cromer_Mann_a4
_atom_type_scat_Cromer_Mann_b4
_atom_type_scat_Cromer_Mann_c
_atom_type_scat_source
'Zn  ' 0.2220 1.4310 14.0743 3.2655 7.0318 0.2333 5.1652 10.3163 2.4100 58.7097
1.3041 International_Tables_Vol_IV_Table_2.2B
'C   ' 0.0020 0.0020 2.3100 20.8439 1.0200 10.2075 1.5886 0.5687 0.8650 51.6512
0.2156 International_Tables_Vol_IV_Table_2.2B
'N   ' 0.0040 0.0030 12.2126 0.0057 3.1322 9.8933 2.0125 28.9975 1.1663 0.5826
-11.5290 International_Tables_Vol_IV_Table_2.2B
'H   ' 0.0000 0.0000 0.4930 10.5109 0.3229 26.1257 0.1402 3.1424 0.0408 57.7997
0.0030 International_Tables_Vol_IV_Table_2.2B
'O   ' 0.0080 0.0060 3.0485 13.2771 2.2868 5.7011 1.5463 0.3239 0.8670 32.9089
0.2508 International_Tables_Vol_IV_Table_2.2B
loop_
_geom_angle_atom_site_label_1
_geom_angle_site_symmetry_1
_geom_angle_atom_site_label_2
_geom_angle_site_symmetry_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
N131 . ZN1 . N31 . 118.34(8) yes
N131 . ZN1 . O11 . 95.05(8) yes
N31 . ZN1 . O11 . 146.48(7) yes
N131 . ZN1 . O12 . 152.81(7) yes
N31 . ZN1 . O12 . 88.74(7) yes
O11 . ZN1 . O12 . 57.79(6) yes
N131 . ZN1 . O21 . 96.93(7) yes
N31 . ZN1 . O21 . 95.65(7) yes
O11 . ZN1 . O21 . 82.34(7) yes
O12 . ZN1 . O21 . 81.66(6) yes
N131 . ZN1 . O10 . 91.41(7) yes
N31 . ZN1 . O10 . 86.67(7) yes
O11 . ZN1 . O10 . 89.76(8) yes
O12 . ZN1 . O10 . 87.62(7) yes
O21 . ZN1 . O10 . 168.96(8) yes
N102 . N101 . C103 2_676 117.8(2) yes
N101 . N102 . C103 . 117.7(2) yes
N101 2_676 C103 . N102 . 124.4(2) yes
N101 2_676 C103 . C133 . 118.2(2) yes
N102 . C103 . C133 . 117.4(2) yes
ZN1 . N131 . C132 . 118.9(2) yes
ZN1 . N131 . C136 . 122.4(2) yes
C132 . N131 . C136 . 118.7(2) yes
N131 . C132 . C133 . 121.7(2) yes
C103 . C133 . C132 . 119.6(2) yes
C103 . C133 . C134 . 121.2(2) yes
C132 . C133 . C134 . 119.2(2) yes
C133 . C134 . C135 . 118.6(2) yes
C134 . C135 . C136 . 119.8(2) yes
N131 . C136 . C135 . 122.1(2) yes
N2 . N1 . C6 . 117.3(2) yes
N1 . N2 . C3 . 117.5(2) yes
N2 . C3 . N4 . 124.8(2) yes
N2 . C3 . C33 . 117.3(2) yes
N4 . C3 . C33 . 117.6(2) yes
C3 . N4 . N5 . 117.5(2) yes
N4 . N5 . C6 . 117.0(2) yes
N1 . C6 . N5 . 125.0(2) yes
N1 . C6 . C63 . 117.6(2) yes
N5 . C6 . C63 . 117.2(2) yes
ZN1 . N31 . C32 . 119.1(2) yes
ZN1 . N31 . C36 . 122.5(1) yes
C32 . N31 . C36 . 118.3(2) yes
N31 . C32 . C33 . 122.4(2) yes
C3 . C33 . C32 . 120.3(2) yes
C3 . C33 . C34 . 121.1(2) yes
C32 . C33 . C34 . 118.5(2) yes
C33 . C34 . C35 . 119.0(2) yes
C34 . C35 . C36 . 119.3(2) yes
N31 . C36 . C35 . 122.5(2) yes
C62 . N61 . C66 . 117.8(2) yes
N61 . C62 . C63 . 122.5(2) yes
C6 . C63 . C62 . 120.7(2) yes
C6 . C63 . C64 . 120.8(2) yes
C62 . C63 . C64 . 118.6(2) yes
C63 . C64 . C65 . 119.1(2) yes
C64 . C65 . C66 . 118.5(2) yes
N61 . C66 . C65 . 123.5(2) yes
O11 . N10 . O12 . 116.8(2) yes
O11 . N10 . O13 . 120.8(2) yes
O12 . N10 . O13 . 122.4(2) yes
ZN1 . O11 . N10 . 95.9(1) yes
ZN1 . O12 . N10 . 89.1(1) yes
O21 . N20 . O22 . 119.7(2) yes
O21 . N20 . O23 . 119.0(2) yes
O22 . N20 . O23 . 121.2(2) yes
ZN1 . O21 . N20 . 117.3(1) yes
ZN1 . O10 . C11 . 131.3(2) yes
loop_
_geom_bond_atom_site_label_1
_geom_bond_site_symmetry_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
ZN1 . N131 . 2.055(2) yes
ZN1 . N31 . 2.080(2) yes
ZN1 . O11 . 2.150(2) yes
ZN1 . O12 . 2.300(2) yes
ZN1 . O21 . 2.125(2) yes
ZN1 . O10 . 2.106(2) yes
N101 . N102 . 1.324(3) yes
N101 . C103 2_676 1.343(3) yes
N102 . C103 . 1.340(3) yes
C103 . C133 . 1.478(3) yes
N131 . C132 . 1.343(3) yes
N131 . C136 . 1.346(3) yes
C132 . C133 . 1.389(3) yes
C133 . C134 . 1.388(3) yes
C134 . C135 . 1.372(4) yes
C135 . C136 . 1.377(3) yes
N1 . N2 . 1.327(3) yes
N1 . C6 . 1.335(3) yes
N2 . C3 . 1.331(3) yes
C3 . N4 . 1.349(3) yes
C3 . C33 . 1.480(3) yes
N4 . N5 . 1.319(3) yes
N5 . C6 . 1.346(3) yes
C6 . C63 . 1.484(3) yes
N31 . C32 . 1.340(3) yes
N31 . C36 . 1.347(3) yes
C32 . C33 . 1.393(3) yes
C33 . C34 . 1.390(3) yes
C34 . C35 . 1.377(3) yes
C35 . C36 . 1.379(4) yes
N61 . C62 . 1.339(3) yes
N61 . C66 . 1.340(3) yes
C62 . C63 . 1.391(3) yes
C63 . C64 . 1.391(3) yes
C64 . C65 . 1.378(3) yes
C65 . C66 . 1.379(4) yes
N10 . O11 . 1.267(2) yes
N10 . O12 . 1.262(3) yes
N10 . O13 . 1.229(3) yes
N20 . O21 . 1.264(3) yes
N20 . O22 . 1.237(2) yes
N20 . O23 . 1.250(3) yes
O10 . C11 . 1.419(3) yes
